**Experimental study on the mix design and fresh properties of **

**concrete**

**Khalid Abdel Naser Abdel Rahim***

Faculty of Civil Engineering, University of Coimbra, Portugal

**ABSTRACT**

This paper is about mix design and fresh properties of concrete. The mix design procedure is a process by which the concrete mix proportions such as cement, water, and aggregates are calculated. This is done by filling the concrete mix design form and going through the five design stages in sequence. The five design stages lead to mix proportions, and from that, the batch weights can be obtained. The fresh properties of concrete consist of testing and noticing concrete properties such as the slump, plastic density, bleeding, segregation, cohesiveness, compactability, and finishability in terms of aggregate type, cement type, amount of fine material, water/cement ratio, and superplasticizer amount required for workability. The manuscript presents experimental testing results of the concrete properties using four different concrete mixes. These are 100% gravel, 100% recycled aggregate, 30% fly ash, and 10% silica fume. The experimental testing was carried out in the concrete laboratory at the University of Dundee.

**Keywords: Concrete mix design, Fly ash, Fresh properties of concrete, Plastic density, Rheumatoid arthritis, Silica fume**
**Submitted: 11-03-2019, Accepted: 22-03-2019, Published: 29-03-2019**

**INTRODUCTION**

**Overview**

The BS 1881: Part 125: 1983 – Testing concrete – Methods for mixing and sampling fresh concrete in the laboratory is set to consider the methods of mixing concrete in terms of sample preparation, mixing, and testing. The testing process included is slump and plastic density test.

In the first section of this report, the mix design procedures will be described along with its five stages and group results. The calculations of the mix design will be shown step by step for the 100% gravel of a 0.45, 0.6, and 0.75 water/cement (W/C) ratio, to obtain the mix proportions for concrete mixes and the batch quantities allowing for absorption.

The mix proportions for concrete mixes of the 100% gravel, 100% recycled aggregate, 30% fly ash/gravel, and 10% silica fume (SF)/gravel will be shown in the form of tables along with the corrected mixes. In addition to this, the batch quantities allowing for absorption tables will be introduced, with some discussion on the reasons of adding extra water.

A step-by-step procedure of the concrete mixing will be presented with the work carried out in the laboratory. Moreover, a brief discussion on the slump and plastic density tests will be introduced in this report. The results of the properties of fresh concrete mix will be commented on, such as aggregate type, cement type, amount of fine aggregate, and W/C ratio.

Finally, as part of the discussion in this report, the yield will be calculated with the corrected mix proportions and difference between design/plastic and volumetric method will be explained.

**Main Aims of the Experimental Study**

The main objectives of the experimental testing were as follows:

• To achieve a better understanding of the concrete mix design process.

• To calculate the mix proportions for concrete mixes and batch quantities allowed for absorption.

• To obtain a greater in-depth knowledge of the mixing procedure and tests carried out in laboratory.

**ISSN Number (2208-6404)**
**Volume 3; Issue 1; March 2019**

**Original Article**

• To become familiar with the fresh properties of concrete. • To be able to correct mix proportions.

• To distinguish between the design/plastic and volumetric method.

• To discussing fresh properties in terms of aggregate type, cement type, amount of fine material, W/C ratio, and the SP amount required for workability.

The major points of the testing were as follows:

• Carrying out mix design for 0.45, 0.6, and 0.75 W/C ratios for uncrushed gravel 100%.

• Calculating batch quantities allowed for absorption. • Mixing concrete according to the building research

establishment mix design.

• Carrying out the slump and plastic density tests.

• Observing the fresh properties of concrete, such as bleeding, segregation, cohesiveness, compactability, finishability, and general overall observation of the mix. • Casting appropriate specimens.

• Curing the specimens as required. • Demolding the specimens after 24 h.

**MIX DESIGN**

**Mix Design Procedures**

The required details for designing concrete mix are cement type, aggregate type, maximum aggregate size, fine aggregate grading, aggregate relative densities, fresh concrete properties, and Hardened concrete properties. The aggregate type used is 100% gravel and three W/C ratios 0.45, 0.6, and 0.75.

The order of concrete mix design procedures consists of five stages as follows:

• Stage 1 is set out to find the free W/C ratio.

• Stage 2 is set out to find the free water content, through
approximate free water contents (kg/m3_{) required to give }

various levels of workability.

• Stage 3 is set out to find the cement content, from equation (1).

*FreeWc*
*FreeW*
*Cc*

*Cr*

= (1)

Where, *Cc* is the cement content, *FreeWc* is the free water
content, *FreeW* is the free water, and *Cr* is the cement ratio.
• Stage 4 is set out to determine the total aggregate content.

First, through estimated wet density of fully compacted concrete to find the concrete density. Second, using equation (2).

*TAc D C W*= − − (2)

Where, *TAc* is the total aggregate content, *D* is the wet density
of concrete (kg/m3_{), }_{C}_{ is the cement content (kg/m}3_{), and }_{W}_{ is }

the free water content (kg/m3_{).}

• Stage 5 is set out to find the fine and coarse aggregate contents. First, through the recommended proportions of fine aggregate according to percentage passing a 600 µm sieve to find the proportion of fine aggregate. Second, using equations (3) and (4), respectively.

*FAc TAc Pf*= × (3)

Where, *FAc* is the fine aggregate content, *TAc* is the total
aggregate content, and Pf is the proportion of fines.

*CAc TAc FAc*= − (4)

Where, *CAc* is the course aggregate content, *TAc* is the total
aggregate content, and *FAc* is the fine aggregate content.

Each of the above stages deals with a particular aspect of the
design, leading to the final mix proportions (kg/m3_{) and the }

batch weights (kg). The factor that has been considered during the mix design is fresh concrete workability, durability, and compressive strength.

**100% Gravel Uncrushed (0.45 W/C Ratio)**

The 0.45 W/C ratio with a cement type of 52.5N, aggregate
type gravel uncrushed, maximum aggregate size 20 mm,
aggregate density of 2600 kg/m3_{, sand density of 2600 kg/m}3_{, }

fine aggregate grading of 44%, and 180 l/m3_{ water content and }

with a slump between 30 and 60 mm.

By applying the mix design procedure, stages stated in Section 2.1, for Stage 1, the free W/C ratio is 0.45 for aggregate type uncrushed 100% gravel and the maximum free W/C ratio using the lower value 0.45 W/C ratio. Stage 2, the free water content slump or Vebe time specified slump is between 30 and 60 mm and the maximum aggregate size specified 20 mm. Accordingly, using the table of approximate free water contents kg/m3

required to give various levels of workability in the engineered
concrete mix design and test methods, the free water content is
180 kg/m3_{. For Stage 3, the cement content using equation 1 is }

400 kg/m3_{ and the modified free W/C ratio is 0.45. Furthermore, }

Stage 4 gives a relative density of the aggregate of 2600 kg/m3

for total aggregate content. Using the appropriate graph for
estimated the wet density of fully compacted concrete, the
concrete density is 2370 kg/m3_{ and the total aggregate content }

using equation 2 equals to 1790 kg/m3_{. Finally, for Stage 5, }

for the fine and coarse aggregate content, the grading of fine
aggregate is 44% for maximum aggregate size of 20 mm, the
proportion of fine aggregate equals 37%. Therefore, using
equation (3), the fine aggregate content is 662 kg/m3_{ and the }

**Mix Proportions for Concrete Mixes**

The same mix design procedure has been carried out for 0.6 and 0.75 W/C ratio and the following Tables 1-4 show how the mix proportions that have been obtained.

**Batch Quantities Allowing for Absorption**

Batch quantities are the quantities of materials such as cement, fly ash, SF, water, recycled aggregate, and aggregates required for a concrete mix process. The batch quantities for the concrete

mixes are presented in Tables 5-8. Moreover, the following equation (5) is used to find the batch quantities allowing for absorption:

*AAbw*=*Abw Aw*− (5)

Where, *AAbw* is the adjusted aggregate batch weight in (kg),

*Abw* is the aggregate batch weight (kg), and *Aw* is the absorbed
water (kg).

The main reason for adding extra water is for absorption of water by the aggregate and due to the characteristics of the aggregate to produce concrete of a specified slump. This depends on the W/C ratio, cement-aggregate ratio, maximum

**Table 1: Mix proportions for 100% gravel**

**Mix proportions, kg/m3**

**Mix W/C **

**ratio** **CEM I** _{Water}_{0/5}Aggregate_{5/10}_{10/20}

0.45 400 180 660 380 750

0.6 300 180 720 390 790

0.75 240 180 820 380 755

Density 3150 1000 2600 2600 2600

W/C: Water/cement

**Table 3: Mix proportions for 100% FA**

**Mix proportions, kg/m3**

**Mix W/C **

**ratio** **CEM I** **FA** _{Water}**Aggregate _{0/5}**

_{5/10}

_{10/20}0.36 355 150 180 560 380 755

0.47 265 115 180 690 375 755

0.59 215 90 180 740 385 770

Density 3150 2250 1000 2600 2600 2600

W/C: Water/cement

**Table 4: Mix proportions for 100% SF**

**Mix proportions, kg/m3**

**Mix W/C **

**ratio** **CEM I** **SF** _{Water}_{0/5}Aggregate_{5/10}_{10/20}

0.45 360 40 180 595 370 735

0.6 270 30 180 685 375 740

0.75 215 25 180 785 360 715

Density 3150 2000 1000 2600 2600 2600

SF: Silica fume, W/C: Water/cement

**Table 5: Batch quantities for 100% gravel**

**Mix proportions, kg/m3**

**Mix W/C **

**ratio** **CEM I** **Water** _{0/5}**Aggregate _{5/10}**

_{10/20}0.45 8 3.89 13.13 7.52 14.85

0.6 6 3.91 14.13 7.72 15.64

0.75 4.8 3.91 16.32 7.52 14.95

W/C: Water/cement

**Table 6: Batch quantities for 100% RA**

**Mix proportions, kg/m3**

**Mix W/C **

**ratio** **CEM I** **Water** _{5/10}**RA _{10/20}**

**Aggregate**

_{0/5}0.45 8 4.4 6.79 13.63 11.94

0.6 6 4.47 6.98 14.02 13.33

0.75 4.8 4.47 6.70 13.35 15.50

RA: Rheumatoid arthritis, W/C: Water/cement

**Table 7: Batch quantities for 100% FA**

**Mix proportions, kg/m3**

**Mix W/C **

**ratio** **CEM I** **FA** _{Water}**Aggregate _{0/5}**

_{5/10}

_{10/20}0.36 7.1 3.0 3.88 11.15 7.53 14.95

0.47 5.3 2.3 3.90 12.90 7.40 15

0.59 4.3 1.8 3.90 14.73 7.62 15.25

W/C: Water/cement

**Table 8: Batch quantities for 100% SF**

**Mix proportions, kg/m3**

**Mix W/C **

**ratio** **CEM I** **SF** _{Water}_{0/5}Aggregate_{5/10}_{10/20}

0.45 7.2 1.6 3.081 11.84 7.325 14.555

0.6 5.4 1.2 3.292 13.015 7.425 14.650

0.5 4.32 0.96 3.414 15.62 7.13 14.155

SF: Silica fume, W/C: Water/cement
**Table 2: Mix proportions for 100% RA**

**Mix proportions, kg/m3**

**Mix W/C **

**ratio** **CEM I** **Water** _{5/10}RA_{10/20}**Aggregate _{0/5}**

0.45 400 180 350 710 600

0.6 300 180 360 730 670

0.75 240 180 345 695 780

Density 3150 1000 2400 2400 2400

aggregate size, and the type, shape, grading, surface texture, absorption capability, strength, and stiffness of aggregate particles. The following equation (6) is used to find the additional water required:

*Awr*=*Mbw Av*− (6)

Where, *Awr* is the additional water required (kg), *Mbw* is the
material batch weight (kg), and *Av* is the absorption value %.

The absorption values for gravel 5/20, sand 0/5, RA 5/10, and RA 10/20 are 1%, 0.5%, 3%, and 4%, respectively.

**Experimental Mixing Procedure and Tests Carried **
**Out**

**Mixing of concrete**

The mixing of concrete was according to BS 1881: Part 125: 1983 – Testing concrete – Methods for mixing and sampling fresh concrete in the laboratory. A lightly dampen mixer pan and paddles have been used to carry out the mixing. First, the following was added in order: Coarse aggregate, fine aggregate, and sand and mixed for 30 s. After that, half of the mix water was added and mixed for another 1 min. Then, the lightly dampen mixer was left covered for 8 min for the aggregates to absorb water. Afterward, the cement was spread evenly over the aggregates and mixed for 1 min. The next step was cleaning the paddles and mix material carefully by hand. Finally, the remaining water (with added superplasticizers) was added to mix and followed by a further mixing for 2 min. Additional hand mixing has been carried out to ensure homogeneity.

**Slump test (Workability)**

The slump test [Figure 1] was according to BS EN 12350-2:2000 – Testing fresh concrete – Part 2: Slump test. First, the inside surface of the slump cone was gently moisten using a damp cloth. After that, the cone was placed on a level surface

and held firmly in position using footrests. Afterward, the slump cone was filled with the freshly mixed concrete in three layers of equal height, using a metal rod each layer has been temped 25 times. The next step was to clean and remove the excess concrete from the top and around the base of the cone. Then, the cone was gently lifted vertically and the cone was inverted and placed next to the slumped concrete. Finally, the vertical distance from the top of the cone to the highest point of the slumped concrete has been measured and all equipments were cleaned.

**Plastic density**

The plastic density test was done according toBS 12350-6, 2000 – Testing concrete – Method for determination of density of compacted fresh concrete. First, the mass of an empty 10 L steel container has been recorded to the nearest 0.01 kg. After that, the container was filled with water so that no meniscus is above the rim. Then, the container was reweighed to obtain mass of water in container to the nearest 0.01 kg. The next step was to empty the container from water and carefully fill it with concrete in six equal layers. Each of the layers has been compacted fully on the vibrating table. Then, the final layer has been smoothed with a float to level with the top container. The next step was to skim the concrete surface with 300 mm steel rule, and the outside of the container has been cleaned thoroughly and reweighed. Finally, the concrete has been returned to the mixer and remixed for 30 s. Plastic density results are demonstrated in Table 9.

After carrying out the mixing of concrete, slump and plastic
density tests, returning, and remixing the concrete for 30 s,
the concrete was casted in 1 cylinder (100 mm × 300 mm in
diameter), 1 prism (100 mm2_{ × 500 mm), 6 cubes (100 mm}3_{), }

and 1 cube (150 mm3_{) for test specimens. In addition, curing of }

the test specimens has been carried out to avoid water loss from the concrete. Finally, the mixer has been cleaned thoroughly and the concrete has been removed from paddles. The casting of the concrete specimens is illustrated in Figure 2.

The calculation for plastic density which was in the concrete laboratory using the formula (7) below:

*m*
*D*

*V*

= (7)

**Figure 1:** Slump measuring and testing

**Table 9: Results for the plastic density test for 100% **
**gravel (kg)**

**Mix, W/C **

**ratio** **empty containerWeight of ** **10 L combinerWith water of ** **concreteWith **

0.45 5.02 11.80 21.335

0.6 5.02 11.80 21.200

0.75 5.02 11.80 21.015

Where, m is mass of concrete in container (to the nearest 10 g)
and *V* is volume of container which is the mass of water in
container (from calibration) divided by 1000 to the nearest
0.00001 m³ equals to 0.01 m³ (approximately).

Accordingly, the plastic density for 0.45 W/C ratio is:

21.335 5.02

2406 kg/m³ 0.0118 0.00502

*D*= − =

−

To the nearest 10 kg/m³ *D* ≈ 2405 kg/m³.

**Yield: Corrected Mix Proportions and Differences **
**between Design/Plastic and Volumetric Method**
**Adjusting for yield**

The yield has been calculated for each of the three W/C ratios 0.45, 0.60, and 0.75 and tabulated in Table 10.

The corrected density has been calculated using equation (8) below:

*ActD*

*CorrD* *eachconstituent*
*TD*

=_{} _{}×

(8)

Where, *CorrD* is the corrected density, *ActD* is the actual
density, and *TD* is the total density.

**Volumetric method**

The reason behind calculating the yield is to find the corrected
mix proportions and comparing the corrected density with
actual plastic density. Moreover, it is calculated to compare the
correction factor of actual and theoretical methods. There are
two types of methods, one is calculated design/plastic and the
other is volumetric method.[1]_{ The volumetric method appears }

to be more efficient and reliable than design/plastic because it

is more accurate and close to actual. In addition, its approach
is more practical and close to real on-site conditions. On the
other hand, the design plastic method is more theoretical and
based on quite a few assumptions, which lead to more errors,
greater time consumption and is difficult to handle.[2]_{ The }

volumetric calculations for 0.45 W/C ratio 100% gravel and corrected gravel are presented in Tables 11 and 12, respectively.

**RESULTS AND COMMENTS ON FRESH **

**PROPERTIES**

**100% Gravel**

The gravel [Table 13] has given the concrete good compactability and finishability apart from 0.45 W/C ratio mix, which had relatively below par. This is due to the shape of the aggregate

**Figure 2:** The picture shows the casting of concrete for testing
specimens

**Table 10: Density, corrected density, and actual plastic **
**density (kg/m3 _{)}**

**Description** **Density** **Corrected** **Actual plastic**

Cement 400 405

Water 180 180

Sand 0/5 660 665

10 aggregate 5/10 380 385 20 aggregate 10/20 750 755

Total 2370 2390 2405

**Table 11: Volumetric tabulated calculation for 0.45 W/C **
**ratio (100%) gravel**

**Description** **0.45 W/C ratio (100% gravel)**
Cement 400 kg/m3_{/3150 kg/m}3_{=0.127}

Water 180 kg/m3_{/1000 kg/m}3_{=0.18}

Aggregates 0/5 660 kg/m3_{/2600 kg/m}3_{=0.254}

Aggregates 5/10 380 kg/m3_{/2600 kg/m}3_{=0.146}

Aggregate 10/20 750 kg/m3_{/2600 kg/m}3_{=0.288}

Actual=0.995 Theoretical=1.000 W/C: Water/cement

**Table 12: Volumetric tabulated calculation for 0.45 W/C **
**ratio (100%) gravel corrected**

**Description** **0.45 W/C ratio (100% gravel) corrected**
Cement 405 kg/m3_{/3150 kg/m}3_{=0.129}

Water 180 kg/m3_{/1000 kg/m}3_{=0.180}

Aggregates 0/5 665 kg/m3_{/2600 kg/m}3_{=0.255}

Aggregates 5/10 385 kg/m3_{/2600 kg/m}3_{=0.147}

Aggregate 10/20 755 kg/m3_{/2600 kg/m}3_{=0.289}

and water absorption value of gravel. Although the concrete had
a cement-rich paste, the Portland cement (CEM I) has worked
sufficiently as a binder between sand and gravel, for a good fresh
concrete with good cohesiveness and compactability.[3] _{The }

amount of sand that has been used was 13.13, 14.33, and 16.32 kg, respectively, for W/C ratios, which seem to be reasonable amounts for the fresh concrete properties for 100% gravel mix. The design mixes of 0.45, 0.6, and 0.75 W/C ratio seem to be acceptable since the slump for each W/C ratio is reasonable and within the required range of 30–60 mm slump. Same applies for plastic density with a good and within range results. In addition, the amount of glenium 51 used was 0.15%, 0.12%, and 0.10% played an important role in preventing bleeding or segregation and improved finishability. In general, the mixes were good and reasonable and with cement-rich paste.

The volume of concrete produced using the equation (9):

*Mc+ Ms + Ma + Mw*
*Vb =*

*D*

(9)

Where, *M _{c}* is batch quantity of cement (kg),

*M*is batch quantity of fine aggregate in laboratory dry condition (kg),

_{s}*M*is batch quantity of coarse aggregate in laboratory dry condition (kg),

_{a}*M _{w}* is batch quantity of mix water (kg), and

*D*is plastic density of fully compacted concrete (kg/m³).

Accordingly, the volume of concrete produced (*Vb*) for
0.45 W/C ratio is:

*8.0kg + 3.89kg + 13.13kg + 7.52kg + 14.85kg*
*Vb =*

*2410 kg / m³*

=0.0197 m3

Where*, V _{b}* has been expressed to an accuracy of 1%, for
example, to the nearest 0.0001 m³ for a 0.01 m³ size mix. The
same calculations have been carried out for 0.6 and 0.75 W/C
ratios and the following Table 14 shows the results.

**100% Recycled Aggregate**

The absorption value for this recycled aggregate was too high;
therefore, it affected the workability by causing high slumps, due
to more water in the mix. For the three W/C ratios, the slump
collapsed with values of 185, 195, and 195 mm, respectively.
However, on the other hand, the use of recycled aggregate
resulted in mix with good compactability and finishability.
Portland cement (CEM I) was added to this mix.[4]_{ The amount }

of Portland cement in this mix was not enough to increase the workability, cohesiveness and inhibit bleeding. In addition, the cohesiveness was poor and there was slight bleeding. The amount of sand in this mix was as follows: 11.94, 13.33, and 15.5 kg in

respect with 0.45, 0.60, and 0.75 W/C ratios. This amount was
not enough to decrease bleeding and reduce segregation and slight
bleeding and segregation were noticed. With an amount of 0.4,
0.6, and 0.75 W/C ratios, it shows from the results that there was
more water in the mix causing high slumps. Moreover, the amount
of glenium 51 used was 0.15%, 0.12%, and 0.10%. Although
this amount of superplasticizer maintained good finishability, it
did not help in improving bleeding and segregation, due to more
water in mix. In general, the absorption value was probably too
high for this RA in Table 15, therefore, leading to more water in
mix, causing high slumps. The density of this recycled aggregate
was probably >2400 kg/m3_{ assumed in design stage and it is more }

likely to be 2550 kg/m3_{.}

General observation/absorption value probably is too high for this RA, therefore, more water in mix causing high slumps and the density of this RA was probably >2400 kg/m³ assumed in design stage. To be more precise the value was about 2550 kg/m³.

**Table 13: Fresh concrete properties for 100% gravel**

**Property** **W/C ratio**

**0.45** **0.6** **0.75**

Slump (mm) 35 55 35

Plastic density (kg/m3_{)} _{2405} _{2385} _{2365}

Bleeding None None None

Segregation None None None

Cohesiveness Good Fair Good

Compactability Fair Good Good

Finishability Fair Good Good

General observation/In my point of view good mixes generally and cement-rich pastes, W/C: Water/cement

**Table 14: Plastic density and volume of concrete **
**produced for 0.45, 0.60, and 0.75 W/C ratio**

**Property** **W/C ratio**

**0.45** **0.6** **0.75**

Plastic density D (kg/m3_{)} _{2405} _{2385} _{2360}

Vb (m3_{)} _{0.0197} _{0.0199} _{0.0201}

W/C: Water/cement

**Table 15: Fresh concrete properties for 100% RA**

**Property** **W/C ratio**

**0.45** **0.6** **0.75**

Slump (mm) 185* 195* 195*

Plastic density (kg/m3_{)} _{2390} _{2375} _{2340}

Bleeding Slight Slight Slight

Segregation Slight Slight Slight

Cohesiveness Poor Poor Poor

Compactability Good Good Good

Finishability Good Good Good

**Table 16. Fresh concrete properties for 30% FA**

**Property** **W/C ratio**

**0.37** **0.45** **0.6**

Slump (mm) 85 ** 190*

Plastic density (kg/m3_{)} _{2470} _{2455} _{2470}

Bleeding None Slight Slight

Segregation None None Slight

Cohesiveness Good Poor Poor

Compactability Good Good Good

Finishability Good Good Good

*Collapsed, **Immediate collapse, general observation/cement-rich mix and too much superplasticizer, W/C: Water/cement

**Table 17: Fresh concrete properties for 10% SF**

**Property** **W/C ratio**

**0.45** **0.6** **0.75**

Slump (mm) 95 80 75

Plastic density (kg/m3_{)} _{2410} _{2375} _{2380}

Bleeding None None None

Segregation None None None

Cohesiveness Good Good Good

Compactability Good Good Good

Finishability Good Good Good

W/C: Water/cement, SF: Silica fume
**30% Fly Ash**

The role of gravel on concrete is that it gives the concrete
good compactability and finishability. Thus, the compactability
and finishability were good for this concrete mix. Portland
cement has reduced bleeding and gave a good cohesiveness in
this mix for 0.37 W/C ratio, but for 0.45 and 0.6 W/C ratios,
there was a slight bleeding and cohesiveness was poor. In
general, it is observed that this mix is a cement-rich mix. The
amount of fly ash added was 3, 2.3, and 1.8 kg in respect with
W/C ratios of 0.36, 0.47, and 0.59. Fly ash is extremely high
fine material. Due to its spherical shape and plain surface of
particles gives it an advantage in terms of water requirement
in concrete mix.[5]_{ The results of fly ash mix as shown in }

Table 16 have improved the compactability of the mix and gave a better finish. Since fly ash is more effective against segregation, it had greater effect on segregation, by having no segregation for both 0.37 and 0.45 W/C ratios and slight segregation for 0.60 W/C ratio. It is believed that the slump for this concrete mix was high with W/C ratios of 0.37, 0.45, and 0.60. The amount of superplasticizer used was 0.30%, 0.33%, and 0.33%, respectively, for the above-mentioned W/C ratios. The above amount of glenium 51 was too much, and thus, chemical reaction did not take place properly in the mix. Therefore, it did not help in producing high workability without segregation or bleeding.

**10% Silica Fume**

In this mix, the gravel has given the fresh concrete good
compactability and finishability. Portland cement (CEM I)
has worked effectively as a binder between sand and gravel,
for a good fresh concrete with good cohesiveness and
compactability. The role of SF on concrete is that it gives
concrete lower permeability by providing unprecedented
reactions in permeability and complete control of bleeding.
Silica fume is an extremely fine and very reactive with spherical
shape particles. Therefore, there is no sign of bleeding in the
mix due to presence of SF. The amount of sand in this mix
was as follows: 12.89, 13.61, and 14.04 kg, respectively, for
0.45, 0.60, and 0.75 W/C ratios. These amounts seem to be fine
since the results of fresh concrete properties were in accord
with the requirement. For 0.45, 0.6, and 0.75 W/C ratio, the
slumps were a bit high with 95, 80, and 75 mm. In addition,
plastic density was fine and within the acceptable range of
2400 kg/m3_{ ± 20 kg/m}3_{. Moreover, the amount of glenium }

51 used was 0.15%, 0.12%, and 0.10%, respectively. These amounts presented reasonable workability with no segregation or bleeding in fresh concrete. Table 17 demonstrates the fresh concrete properties for 10% SF.

**CONCLUSION**

Having completed this experimental study, new aspects have been learned, such as calculating a concrete mix design to obtain mix proportions and batch weights. Mixing concrete with accordance to BS 1881: Part 125: 1983 – Testing concrete – Methods for mixing and sampling fresh concrete in the laboratory and carrying out slump and plastic density tests. In addition, it is found that the amount of water absorbed by the aggregate depends on many factors such as W/C ratio, cement-aggregate ratio, maximum aggregate size, and the type, shape, grading, surface texture, absorption capability, strength, and stiffness of aggregate particles. Moreover, the volumetric method found to be more effective than design/plastic method because it is more accurate and close to actual. Furthermore, it is observed that the fresh properties of concrete are affected by many factors such as aggregate type, cement type, amount of fine material, W/C ratio, and amount of superplasticizer added to mix.

The results of 100% gravel established a good concrete mix.
The slump expressed good workability by presenting acceptable
and within range results between 30 and 60 mm. Moreover,
the result for plastic density was fine with values of 2405,
2385, and 2365 kg/m3_{. In addition, there was no bleeding or }

the usage in the construction site. Such improvements may be by reducing the amount of cement in the concrete mix.

**REFERENCES**

1. Day KW. Concrete Mix Design, Quality Control, and Specification. London, New York: E and EN Spon; 1999. 2. Kett I. Engineered Concrete: Mix Design and Test Methods.

Boca Raton: CRC Press/Taylor and Francis; 2008.

3. Bye GC, Institute of Ceramics Great Britain. Portland Cement: Composition, Production, and Properties. Oxford [Oxford Shire],

This work is licensed under a Creative Commons Attribution Non-Commercial 4.0 International License.

New York: Pergamon Press; 1983.

4. Bartos P. Rilem Technical Committee TC 145 Workability of Special Concrete Mixes and Rilem Technical Committee TC 150 Efficiency of Concrete Mixers. (1994) Special Concretes: Workability and Mixing: Proceedings of the International RILEM Workshop Organized by RILEM Technical Committee TC 145, Workability of Special Concrete Mixes, in Collaboration with RILEM Technical Committee TC 150, Efficiency of Concrete Mixers, and held at the University of Paisley, Scotland. London, New York: E and FN Spon; 1993.